HAL Id: hal-01820675
Submitted on 22 Jun 2018
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Improvement of electrochemical performances of
catechol-based supercapacitor electrodes by tuning the
redox potential via different-sized O-protected catechol
Ewen Touzé, Frédéric Gohier, Barbara Daffos, Pierre-Louis Taberna, Charles
To cite this version:
Ewen Touzé, Frédéric Gohier, Barbara Daffos, Pierre-Louis Taberna, Charles Cougnon. Improvement
of electrochemical performances of catechol-based supercapacitor electrodes by tuning the redox
po-tential via different-sized O-protected catechol diazonium salts. Electrochimica Acta, Elsevier, 2018,
vol. 265, pp. 121-130. �10.1016/j.electacta.2018.01.115�. �hal-01820675�
This is an author-deposited version published in :
Eprints ID : 20194
To link to this article : DOI:10.1016/j.electacta.2018.01.115
To cite this version : Touzé, Ewen and Gohier, Frédéric and Daffos,
and Taberna, Pierre-Louis
and Cougnon, Charles
Improvement of electrochemical performances of catechol-based
supercapacitor electrodes by tuning the redox potential via
different-sized O-protected catechol diazonium salts. (2018) Electrochimica
Acta, vol. 265. pp. 121-130. ISSN 0013-4686
Any correspondence concerning this service should be sent to the repository
OATAO is an open access repository that collects the work of Toulouse researchers and
makes it freely available over the web where possible.
Improvement of electrochemical performances of catechol-based
supercapacitor electrodes by tuning the redox potential via
different-sized O-protected catechol diazonium salts
, Frederic Gohiera
, Barbara Daffosb,c
, Pierre-Louis Tabernab,c
aLaboratoire MOLTECH-Anjou, Universite d’Angers, UMR CNRS 6200, 2 bd Lavoisier, 49045, Angers Cedex, France bCIRIMAT, Universite de Toulouse, UMR CNRS 5085, INPT, UPS, 118 Route de Narbonne, 31062, Toulouse Cedex 09, France cReseau sur le Stockage Electrochimique de l'Energie (RS2E), FR CNRS 3459, 33 Rue Saint Leu, 80039, Amiens Cedex, France
Keywords: Energy Supercapacitors Diazonium salts Microporous carbon Catechol
a b s t r a c t
Two different O-protected catechol diazonium salts were synthetized and reacted with microporous Norit-S50 carbon to investigate the impact of the protecting group on the electrochemical performances of supercapacitor electrodes in 1 M H2SO4. Carbon products were characterized by thermal gravimetric
analysis (TGA), X-ray photoelectron spectroscopy (XPS) experiments and nitrogen gas adsorption-desorption measurements to investigate theﬁlm composition, as well as the impact of the grafting on the textural properties of the Norit-S50. Supercapacitor electrodes, prepared from carbon products, were studied by cyclic voltammetry at different scan rates and by galvanostatic charge/discharge experiments after deprotection of catechol-attached groups. It was found that the speciﬁc charge was improved by introducing catechol groups under protected forms and that the potential at which the redox reaction occurred depends on the protecting group used. With bulky triisopropylsilyl protecting groups, the formal potential of catechol-attached moieties shifted in the positive direction by about 300 mV, yielding an energy gain signiﬁcantly increased, compared to the same charge stored in the level of catechol groups introduced with methyl protecting groups. 1100 repetitive charge/discharge curves at 1 A g1 were achieved to study the stability of supercapacitors electrodes. Results obtained were tentatively explained in terms of the porous structure of the carbon.
Faradaic-based systems for pseudosupercapacitors are touted for their charge storage and power potentialities, promoted by a reversible surface redox reaction [1,2]. In particular, carbon elec-trodes grafted with small redox molecules have been proposed to increase capacitance beyond the double-layer charge storage pro-cess, while avoiding the release of molecules towards liquid elec-trolytes [3e16]. Despite a growing interest in this ﬁeld, these carbon-molecules hybrid systems suffer from a low energy den-sity delivery at the discharge, due to the redox potential often located far away from the electrochemical stability limits of the liquid electrolytes. In contrast to capacitive systems, the design of
faradaic materials at a molecular scale is a promising direction to tackle this issue. A proper selection of electroactive molecules al-lows maximizing the energy stored in the system by positioning their formal potential near to the low or high limit of the potential window, because the energy increases with the square of the voltage. This is especially true for dual-redox asymmetric systems where both positive and negative electrodes are modiﬁed, because the electrochemical storage at the level of molecules ideally should occurs with high voltage swings [17e20]. Different approaches have been developed to predict the formal potential of molecules and identify promising candidates for storage applications [21e24]. It was found that addition of aromatic rings, electron-donating or electron-withdrawing groups and heteroatoms have an impact on the formal potential of redox molecules. However, the preparation of selected molecules is rapidly becoming expensive and time consuming. Importantly, it is well-known that the location of the peak potential in cyclic voltammetry depends also on the relative
strength of the adsorption of oxidized and reduced forms of redox molecules. Accordingly, when an electroactive molecule is grafted on porous carbons, a strong anisotropy in surface reactivity con-tributes to the characteristic multi-peak cyclic voltammograms [18,25]. In the literature, such splitting of the peak potential is often attributed to the presence of different energetically favorable binding surface sites due to the presence of different chemical surface functionalities or structural defects, especially for the catechol unit that is expected to diffuse into the pores [26e30]. In the cyclic voltammograms of catechol-modiﬁed porous carbon electrodes, two major pairs of symmetric peaks typically separated by about 200 mV are generally obtained [28e30]. In these studies, theﬁrst reversible electrochemical system at lowest potentials was attributed to molecules introduced within the microporous surface, while the reversible system shifted in the positive direction cor-responds to molecules located outside of the microporosity. By assuming that it could be possible to selectively introduce mole-cules on the external surface, this splintering of the peak potential could be a simple and universal remedial solution to the limitations of energy density for supercapacitors, especially in aqueous elec-trolytes where the electrochemical stability potential window is limited.
Here, we propose to prevent molecules from entering into the micropore structure of the carbon by increasing the relative size of catechol moieties with encumbering substituents, in order to obtain a redox material modiﬁed only on the outer surface where molecules are redox active at the higher potential after depro-tection. This protection/deprotection strategy will be illustrated with methyl and silyl protective groups due to their facile electro-chemical deprotection [9,31]. Catechol derivatives were immobi-lized on the microporous Norit carbon by spontaneous reaction with the corresponding diazonium salts and carbon products were characterized by TGA analysis, XPS experiments and nitrogen gas adsorption-desorption measurements in order to provide infor-mation about theﬁlm composition, as well as the impact of the grafting on the textural properties of the porous carbon. Super-capacitor electrodes prepared from carbon products were studied by cyclic voltammetry and galvanostatic charge/discharge experi-ments in aqueous electrolyte in order to study the impact of the protecting group on their performances.
2. Experimental 2.1. Reagents and surfaces
3,dimethoxyaniline (98%) was purchased from Alfa Aesar,
4-nitrocatechol (97%), triisopropylsilyl chloride (97%), boron tri-ﬂuoride etherate (46% BF3basis) and boron tribromide (99.99%)
from Aldrich, imidazole (95%) from Fluka and tert-butylnitrite (90%) was received from ACROS. Tetrabutylammonium hexa-ﬂuorophosphate (Aldrich) and acetonitrile (HPLC grade, Carlo Erba) were used as received. Carbon powder (Norit-S50) was obtained from Norit. Glassy carbon (GC) electrodes from Bioanalytical Sys-tems Inc. (model MF-2012; 3 mm in diameter) were used for cyclic voltammetry.
2.2. Synthesis of aryldiazonium salts
The general procedure for the synthesis of aryldiazonium salts is described in Scheme 1 and follows synthetic routes previously published [32,33].
3,4-dimethoxybenzenediazonium tetraﬂuoroborate (1). Boron triﬂuoride etherate (9.79 mmol, 1.5 equiv.) was added to a solution of 3,4-dimethoxyaniline (6.53 mmol, 1 equiv.) in 20 mL of THF at an ice bath temperature. After 5 min stirring, tert-butylnitrite (7.83 mmol, 1.2 equiv.) was added drop wise at 0C. After 15 min stirring, the precipitated was ﬁltered and washed with diethyl ether to afford the diazonium salt in 90% yield as a black powder.
1H NMR (300 MHz, (CD 3)2CO, TMS):
d¼ 8.55 (dd, 3J (H,H)¼ 9.1 Hz,4J (H,H)¼ 2.5 Hz, 1 H), 8.22 (d,4J (H,H)¼ 2.5 Hz, 1 H), 7.56 (d,3J (H,H)¼ 9.0 Hz, 1H), 4.17 (s, 3H), 3.99 (s, 3H).13C NMR (100 MHz, (CD3)2CO):
d¼ 161.7, 151.2, 131.9, 114.4, 113.4, 103.2, 57.8, 57.3.
3,4-dihydroxybenzenediazonium tetraﬂuoroborate (2). 3,4-dimethoxybenzenediazonium tetraﬂuoroborate (1) (1 mmol, 1 equiv), was dissolved in 3 mL of toluene under argon atmosphere. Then 1 M boron tribromide in CH2Cl2(3 mmol, 3 equiv) was slowly
added at room temperature to the solution and the mixture was stirred for 1 h at 40C. After cooling, MeOH (1 mL) was added. After 5 min stirring, the mixture was concentrated under reduced pres-sure to give a dark residue, which was recrystallized from meth-anol/ether. The product was obtained in 84% yield as a brown powder. 1H NMR (300 MHz, D 2O, TMS):
d¼ 8.06 (dd,3J (H,H)¼ 9.0 Hz,4J (H,H)¼ 2.6 Hz, 1 H), 7.79 (d, 4J (H,H)¼ 2.6 Hz, 1 H), 7.18 (d, 3J (H,H)¼ 9.0 Hz, 1H).13C NMR (100 MHz, (CD 3)2CO):
d¼ 161.9, 148.9, 130.7, 118.9, 117.3, 100.1. 3,4-bis((triisopropylsilyl)oxy)benzenediazonium tetra-ﬂuoroborate (3). A solution of 4-nitrocatechol (7.48 g, 1 equiv.), triisopropylsilyl chloride (18.67 mmol, 2.5 equiv.), imidazole (19.10 mmol, 2.55 equiv.) and dimethylaminopyridine (DMAP; 0.67 mmol, 0.1 equiv.) in DMF (36 mL) was stirred at room
temperature for 16 h. The reaction solution was poured into water (50 mL) and extracted with EtOAc (2 50 mL). The organic layers were combined and washed with water (2 50 mL), dried over Na2SO4,ﬁltered and concentrated under vacuum to an orange oil.
The crude reaction mixture was puriﬁed via SiO2chromatography
(gradient 0e10% EtOAc in hexane) to afford the triisopropylsilyl protected nitrocatechol as a pale yellow solid in 86% yield. A sus-pension of triisopropylsilyl protected nitrocatechol (5.99 mmol, 1 equiv.) and 10% palladium on carbon (0.64 g, 0.60 mmol) in ethanol (40 mL) was evacuated andﬂushed with hydrogen gas (1 atm). The suspension was stirred under nitrogen atmosphere for 24 h at 40C. The reaction mixture was then evacuated,ﬂushed with argon and then ﬁltered through celite (50 g) with dichloromethane (200 mL). The ﬁltrate was concentrated under vacuum and the resulting crude oil was puriﬁed via SiO2with dichloromethane to
afford compound 3 in 75% yield as a yellow solid. 1H NMR (300 MHz, (CD3)2CO, TMS):
d¼ 7.45 (d,3J (H,H)¼ 9.0 Hz, 1 H), 6.96
(d, 3J (H,H)¼ 9.0 Hz, 1 H), 6.13 (s, 1 H), 1.31 (m, 36 H). 13C NMR
(75 MHz, CDCl3):
d¼ 162.4, 145.8, 130.9, 120.3, 118.4, 99.2, 17.2, 11.7.
2.3. Chemical modiﬁcation of glassy carbon and activated carbon Before modiﬁcation, glassy carbon electrodes were polished using 0.04
mm alumina and next, sonicated in water and acetoni-trile. Glassy carbon working electrodes were electrochemically modiﬁed in 1 mM acetonitrile solutions of diazonium salts þ0.1 M Bu4NPF6 by recording 10 successive cyclic voltammograms (CVs)
from 0 V to0.7 V vs. Ag/AgNO3at 100 mV s1. After sonication in
acetonitrile and water, modiﬁed electrodes were studied by cyclic voltammetry at 100 mV s1in 0.1 M H2SO4. In aqueous electrolyte,
the electrode potential is referred to the Ag/AgCl system.
For the modiﬁcation of the carbon powder, 400 mg of carbon Norit-S50 (NS) was dispersed in 50 mL of acetonitrile by sonication for 30 min and then 1.67 mmol (0.05 equivalent versus carbon) of diazonium salts was added. After stirring at room temperature for 5 h, the reaction mixture was vacuumﬁltered on a Teﬂon ﬁltration membrane (from Sartorius Stedim) having a pore size diameter of 0.2
mm Carbon products obtained were thoroughly washed twice with acetonitrile (100 mL), DMF (100 mL), methanol (100 mL) and acetone (100 mL), before to be dried overnight at 80C.
2.4. Preparation of supercapacitors electrodes
Supercapacitors electrodes were prepared by mixing the active material with polytetraﬂuoroethylene (PTFE, 60 wt% dispersion in water) used as binder and carbon black (superior graphite) used as conducting additive with a ratio of 75:10:15 (wt; wt; wt) in a small volume of ethanol until a homogeneous carbon paste was obtained. The carbon paste was spread to obtain a thinﬁlm which was dried at 80C for 1 h. A sample of some milligrams was pressed for 60 s at 1 MPa between two stainless steel grids (80 mesh, 0.127 mm, Alfa Aesar) used as current collector.
Electrochemical measurements were achieved at room tem-perature in a three-electrode cell connected to a potentiostat/gal-vanostat model VSP (from Bio-Logic) monitored by ECLab software. XPS measurements were performed with a Kratos Axis Ultra spectrometer using a Al Ka monochromatic beam working at 1486.6 eV. All spectra were recorded in the constant energy mode at a pass energy of 20 eV. Data treatment was performed with CasaXPS software and all spectra were calibrated taking 284.5 eV (graphite like carbon) as a reference binding energy. Porosity characteristics were calculated from nitrogen sorption isotherms
measured at 77 K using a Micromeritics ASAP 2020 porosimeter. The speciﬁc surface area was estimated by using BET, while the pore volumes and the pore size distributions were calculated from adsorption isotherms by using the QSDFT method. TGA analyses were performed using a TA instruments (TGA Q500) apparatus by heating 5 mg typical masses of carbon products in nitrogen atmo-sphere from 60C to 1200C at a rate of 10C/min. The tempera-ture was maintained at 60C for 20 min before the experiment starts.
3. Results and discussion
3.1. Spontaneous grafting of the aryldiazonium salts on Norit S50
Fig. 1shows XPS spectra of the C1s and N1s core levels for un-modiﬁed and functionalized Norit carbon products.
Beside a main photoelectron peak at 284.5 eV that is assigned to sp2 CeC bonds in graphite-like carbon, the C1s XPS spectra of modiﬁed carbons show photoemission peaks at higher binding energies, which are attributed to electron deﬁcient carbon atoms. C1s XPS spectra for the Norit carbon modiﬁed with the 3,4-dihydroxybenzenediazonium salt and the 3,4-dimethoxybenzenediazonium salt correlate well with two contri-butions at around 286 eV and 287 eV in addition to the reference peak at 284.5 eV. The peak at 286 eV can be assigned to the CeOH and CeOeC contributions depending on whether catechol or dimethoxybenzene units were introduced [16,34,35]. The peak at 287 eV might originate from carbonyl functionalities present at the surface of the pristine Norit carbon or can provide from partial oxidation of catechol groups . For the Norit carbon modiﬁed with the 3,4-bis((triisopropylsilyl)oxy)benzenediazonium salt, two additional contributions were obtained at 283.5 eV and 285.3 eV, which can be attributed to the CeSi bond and sp3-hybridized
car-bons providing to the silyl protecting groups . A peak at 101.5 eV in the XPS spectrum of the Si2p core level also provides evidence of the introduction of bis((triisopropylsilyl)oxy)benzene units (Fig. S1) .
The N1s core-level spectra show nitrogen contributions over a wide range of binding energy, corresponding to nitrogen species in high and low oxidation states. Note that the unmodiﬁed carbon does not show any nitrogen peaks, conﬁrming that the pristine carbon does not contain detectable nitrogen species. The presence of N1s emission for carbons modiﬁed with diazonium salts that do not bear any nitrogen-containing substituent, is frequently re-ported in literature, proving that the dediazoniation step is uncomplete during the grafting process . The peak at around 400 eV has been assigned to diazenyl groups resulting to the elec-trophilic attack of the diazonium cation on the carbon surface or on the phenyl ring of previously attached molecules [38e40]. At 399 eV and 402 eV, two additional peaks were detected, which can be attributed to physisorbed ACN and DMF molecules used as rinsing solvents . At higher binding energies, the presence of two peaks at 404.8 eV and 406.4 eV with an area ratio of 1:1 is characteristic of diazonium groups [42e44]. The peak at the high-est binding energy is assigned by Finn and Jolly to the nitrogen atom directly attached to the phenyl group in the diazonium salt . These peaks may be assigned to strongly physisorbed diazo-nium salts, forming complexes with aromatic structures . This explanation is well supported by the presence of F1s and B1s peaks in the wide XPS survey spectrum of the Norit carbon modiﬁed with the 3,4-bis((triisopropylsilyl)oxy)benzenediazonium tetra-ﬂuoroborate (Fig. S2).
Importantly, with the silyl protecting groups, the N1s peak attributed to azo-bonds became prominent compared to the other carbon products. This is possibly due to a more efﬁcient formation
of azo-bonds with the 3,4-bis((triisopropylsilyl)oxy)benzenedia-zonium salt. Nevertheless, this seems unlikely to be able to fully account for the very marked differences in the N1s XPS spectra, because the electrophilic attack of diazonium cations is mainly governed by their electronic properties , which do not signi ﬁ-cantly change when the oxygen atoms are protected with methyl or silyl groups. A more tenable explanation is that the molecules protected with bulky silyl groups are selectively introduced on the outer surface of the Norit carbon and become more“visible” by the surface-sensitive XPS measurements .
3.2. Electrochemical behavior of modiﬁed Norit carbon electrodes
Fig. 2shows CVs recorded in 1 M H2SO4on Norit carbon
elec-trodes spontaneously modiﬁed with the three diazonium salts
studied. Note that before study, the surface-attached molecules were electrochemically deprotected by recording successive CVs in 1 M H2SO4up to 0.8 V until a stabilized CV was obtained . In this
way, after deprotection, a catechol-tethered surface is obtained whatever the diazonium salt used. However, the different locations in potential of the electrochemical systems ascribed to the attached-catechol moieties and their relative intensities, indicate a possible effect of the protecting groups on the selectivity and the efﬁciency of the surface grafting process.
CVs obtained shows two reversible systems separated by about 300 mV, possibly due to catechol moieties in different chemical environments. Nagaoka and Yoshino observed a similar complex CV for the catechol adsorbed on an anodized GC electrode (the anodic treatment creates microporosity) . Authors conclude that the more anodic reversible system corresponds to adsorption Fig. 1. XPS spectra of C1s and N1s core levels for unmodiﬁed (a) and modiﬁed Norit carbon with 3,4-dihydroxybenzenediazonium salt (b), 3,4-dimethoxybenzenediazonium salt (c) and 3,4-bis((triisopropylsilyl)oxy)benzenediazonium salt (d).
of catechol on the outer surface, while the reversible system shifted towards the negative direction arises from catechol adsorbed on the micropore surface. Authors evoke a favorable
pinteraction between catechol and graphite-like surface of glassy carbon required to enter into the microporosity.
From our results, only the Norit carbon modiﬁed with the 3,4-dihydroxybenzenediazonium salt give two well-deﬁned revers-ible systems of almost equal current intensity (Fig. 2a). After modiﬁcation with 3,4-dimethoxybenzenediazonium salt, the ﬁrst reversible system dominates (Fig. 2b), while mainly the second system contributes to the faradaic envelope of the CV recorded with the Norit electrode modiﬁed with 3,4-bis((triisopropylsilyl)oxy) benzenediazonium salt (Fig. 2c). These differences can be tenta-tively explained in terms of the porous structure of the Norit carbon if we assume that the pores diameter is too small for the O-pro-tected catechol diazonium salt with bulky silyl groups, while catechol and dimethoxybenzene derivatives can diffuse in the porous structure.
The total speciﬁc charge (QT), determined by integrating the
area under the CVs presented inFig. 2and the faradaic contribution (QF) of molecules to the charge storage, deduced by subtracting the
double-layer contribution (Qdl) of the carbon, are showed inTable 1
for all carbon products. In addition, determination of the molecule-loading (
GTGA) by TGA experiments in N2atmosphere, gives access
to the faradaic efﬁciency of molecules by assuming that two elec-trons per molecule were exchanged.
Despite QTis improved in all cases after modiﬁcation, QFvaries
in the order Norit-OTIPS> Norit-OME > Norit-OH, while the molecular-loading shows the opposite, implying a better faradaic efﬁciency of molecules for Norit-OTIPS. Note that the double-layer of the Norit carbon is weakly impacted by the grafting whatever the diazonium salt used. With Norit-OTIPS, the more important frac-tion of molecules involved in the charge storage process is consis-tent with an improved electrochemical accessibility of molecules, while the important fraction of“silent” molecules with Norit-OH and Norit-OMe can be considered as a“dead mass” due to their isolation in the porous structures of the carbon. To verify this assumption, CVs were recorded at different scan rates comprised between 7 mV s1and 150 mV s1.Fig. 3shows the variation of the total speciﬁc charge as a function of scan rate. For the unmodiﬁed Norit electrode, a rapid increase of QTis noticeable at slow scan rate
(<20 mV s1), due to a larger fraction of the speciﬁc area accessible to ions at this time scale. For supercapacitor electrodes prepared from Norit-OH and Norit-OMe, QTis less inﬂuenced by the scan rate
in the low scan rate domain, which is indicative of a poorer accessibility of ions to the micropore surface. With the Norit-OTIPS, the scan rate dependence of the total speciﬁc charge over the low scan rate domain follows approximately the same trend that for the unmodiﬁed Norit electrode, implying that no signiﬁcant obstruc-tion of porosity occurs during the chemical modiﬁcation of the carbon. By analogy, a previous work reported by Hapiot et al. may provides guidance for interpretation of the scan rate effect on the speciﬁc charge . Authors have demonstrated that the use of diazonium salts with functionalities protected by different-sized groups allows to ﬁnely control the structure of a molecular as-sembly at a surface, obtaining molecules spaced away from each other with a gap created by the release of protecting groups. Especially, the use of bulky protecting groups, such as triisopro-pylsilyl groups, was found to increase the permeability of the organic layer by creating diffusion channels in the layer after deprotection. In our case, it can be assume that the use of triiso-propylsilyl protecting groups improves the electrolyte penetrability in the porous structure of the carbon by avoiding molecules to enter into the micropores of diameter less than the molecular size and by restoring diffusion channel through the layer after deprotection.
However, there is not a clear consensus on which effect (i.e., textural effect or chemical effect) is responsible to the multi-peak features of the CVs. Interestingly, when a glassy carbon electrode polished to a mirror-like appearance was modiﬁed by electro-chemical reduction in acetonitrile solutions containing the diazo-nium salts studied, the grafting, which is assumed to occurred by radical attack, produced in all cases a main reversible electro-chemical system centered at 0.55 V vs. Ag/AgCl (Fig. S3), implying that the porous interface could be responsible to the multi-peaks system obtained with modiﬁed Norit electrodes. From the simi-larities between the reversible system obtained with a perfectlyﬂat modiﬁed glassy carbon electrode and the second system observed with modiﬁed Norit electrodes, it seems reasonable to propose that this latter system can be ascribed to molecules grafted by radical attack on the outer surface or at the micropores entrance. In this way, a tenable explanation for the multi-peak CVs obtained with modiﬁed Norit electrodes is that molecules introduced on the in-ternal surface of the porous interface could be responsible for the ﬁrst reversible system. This explanation is reinforced by a recent work of Downard et al. evoking the possibility of a spontaneous grafting mechanism in two steps, includingﬁrst the formation of a primer organic layer on the surface by radical attack and second, the further growth of this organic layer by reaction with a solution-generated reactive species . If a similar mechanism operates in this work, a process involving surface attack by radicals can account for the spontaneous grafting reaction at short reaction times. 3.3. Impact of the chemical modiﬁcation on the textural properties of the Norit carbon
To investigate in detail the impact of the grafting on the textural properties of the Norit carbon, nitrogen gas adsorption-desorption measurements were achieved with unmodiﬁed and modiﬁed car-bons (Fig. 4).
Before chemical modiﬁcation, the adsorption branch of the isotherm of the Norit carbon presents a net increase in the adsor-bed volume at low relative pressure (P/P0) followed by a nearly horizontal plateau in the intermediate and high P/P0values, while the desorption branch of the isotherm retraces nearly the same path. Such N2 adsorption-desorption isotherms approach a
reversible type I isotherm, according to the IUPAC classiﬁcation, which is typical of a microporous structure . After chemical modiﬁcation, the adsorption-desorption isotherms of the Norit carbon show a net decrease in the adsorbed volume at low relative pressure. The loss of adsorbed volume is becoming more pro-nounced with protected molecules and increases in the order Norit-OH< Norit-OMe < Norit-OTIPS. With unprotected catechol, the BET speciﬁc surface area reduced from 1699 m2g1 to
1349 m2g1, while it reduced up to 1158 m2g1and 1113 m2g1 with methyl and triisopropylsilyl protective groups, respectively. These results demonstrate that the microporous surface is differ-ently impacted by the grafting, depending on the molecular sizes. Especially, a more important fraction of micropores is suppressed as the molecular size increases, implying that the grafting mainly blocks the microposity by a steric effect. For better understanding the impact of the grafting on the carbon texture, isotherms were further analyzed by determining the pore size distribution (Fig. 5). Before chemical modiﬁcation, the pore size distribution shows that the Norit carbon has mainly micropores (<2 nm) with a small fraction of mesopores between 2 and 2.5 nm. After grafting, the pore size distribution in the micropores domain is differently impacted according to the diazonium salt used, while the loss of the mesopores volume is nearly the same. Such results support that the microporosity is responsible to the complex CVs obtained with modiﬁed Norit electrodes. Intriguingly, with the bulky silyl
protecting groups, the larger micropores with 1.5e2 nm diameter are less impacted by the chemical modiﬁcation, compared to the methyl protecting groups. Assuming that the accumulation of molecules at the entrance of micropores is responsible to the loss of the microporous volume, an increase in the size of molecules is expected to favor such “constriction” phenomenon . On the contrary, for the mesopores, a progressive coverage of the inner pore surface is expected to give a more progressive decrease of their volume and so, mesopores are expected to be less sensitive to the molecular size. To compare the affected pore region for the two O-protected catechol carbon products, which give a different location in potential for the main reversible system in cyclic vol-tammetry, the inset ofFig. 5presents the subtracted pore volume distribution obtained by difference between the pore size distri-bution for the bis((triisopropylsilyl)oxy)benzene and dimethoxybenzene-modiﬁed Norit carbons. Assuming that the accumulation of molecules at the pore entrance is preferred, there is tentative evidence from the data inFig. 5that with pores having diameters below 0.6 nm, both the dimethoxybenzene and the bis((triisopropylsilyl)oxy)benzene units are large enough for blocking pores by the grafting of a single molecule at their entrance, while the grafting of silyl protected molecules more efﬁciently blocks pores with 0.60e1.35 nm diameter. In contrast, pores with diameter larger than 1.35 nm were found to be less obstructed by the bis((triisopropylsilyl)oxy)benzene units, compared to the dimethoxybenzene-modiﬁed Norit carbon. These changes ﬁt well with the molecular sizes regarded as the higher interatomic dis-tance between the two protecting groups. Molecular sizes were calculated by Chem3D and found to be 0.59 nm with the methyl groups and 1.2 nm with the silyl groups. InFig. 6, we propose to normalize the pore size distribution of the Norit carbon by the molecular size. With such normalized pore size distribution, it appears that the Norit carbon has mainly pores with diameters less than two times the size of bis((triisopropylsilyl)oxy)benzene units. For pores with a diameter corresponding to the size of mole-cules, accumulation of molecules at their entrance immediately blocs their access to N2adsorbate, while pores with normalized
diameter comprise between 1 and 2 remain accessible to the adsorbate but do not allow the diffusion of molecules inside the porosity. Only pores with normalized diameter more than 2, can be accessed by molecules and can be possibly modiﬁed on their inner surface. Such representation permits to rationalize results and suggests that the porosity must be adapted to the molecular size. With this approach, it would be expected that the 3,4-bis((triisopropylsilyl)oxy)benzenediazonium salt mainly affects the outer surface of the Norit carbon, while the 3,4-dimethoxybenzenediazonium salt can have access to a part of the micropore volume, which can be possibly reduced by a progressive coverage of their inner surface. This explanation supports that the different locations in potential of the reversible electrochemical systems obtained in cyclic voltammetry are mainly due to a textural effect and it was found that a higher energy corresponds to the electric charge stored at the level of molecules grafted at the pores entrance. In this way, this protection/deprotection strategy offers the possibility of matching a more important energy to the faradaic contribution of the electric charge storage by adjusting the mo-lecular sizes to the textural properties of the carbon.
3.4. Impact of the protecting group on the energy density of supercapacitors
In order to evaluate the beneﬁt of the protecting groups on the electrochemical performances of modiﬁed-carbon based super-capacitors electrodes, galvanostatic charge/discharge experiments were performed from 0 to 0.8 V at 1 A g1.Fig. 7A presents the Fig. 2. CVs recorded at 10 mV s1in 1 M H2SO4with unmodiﬁed Norit carbon
elec-trode (curve in dotted line) and with Norit carbon elecelec-trodes modiﬁed with 3,4-dihydroxybenzenediazonium salt (a), 3,4-dimethoxybenzenediazonium salt (b) and 3,4-bis((triisopropylsilyl)oxy)benzenediazonium salt (c). The current was normalized with respect to the mass of active material (without organic binder and superior graphite).
discharge curves andFig. 7B shows the evolution of the total spe-ciﬁc charge QTdeduced to the charge/discharge curves at 1 A g1
during theﬁrst 1100 cycles.
Dt corresponds to the average speciﬁc charge, the increase in charge/discharge time for modiﬁed carbons is indicative of an increase in the global speciﬁc charge. After modiﬁcation with catechol derivatives a speciﬁc charge gain comprised between 20% and 30% is obtained. Note that the two carbon products Norit-OH and Norit-OMe give nearly the same increase in speciﬁc charge, while the most signiﬁcant improvement corresponds to Norit-OTIPS, in good agreement with the CVs.Fig. 7B shows that, in all
cases, the speciﬁc charge slightly decrease during the ﬁrst few hundred cycles, due to the departure of just physisorbed molecules from the surface to the liquid electrolyte, and then tends to stabilize after 1000 charge/discharge cycles, indicating that the beneﬁcial effect of the catechol groups remains even after long time cycling. The speciﬁc charge retention after 1000 cycles is 89.4% for Norit-OH, 95.4% for Norit-OMe and 89.6% for Norit-OTIPS. Note that carbon products where molecules or a fraction of molecules are suspected to be grafted onto the external surface have depressed charge retentions, probably due to a better contact between mol-ecules and the liquid electrolyte that favours their desorption. For the same reason, the excellent charge retention obtained with Norit-OMe can be explained by a poorer contact between mole-cules and the liquid electrolyte, due to their isolation in the microporosity.
Importantly, the potential at which the redox reactions occur change depending on the diazonium salt used for the chemical modiﬁcation. With O-methyl protected catechol moieties, a plateau is clearly visible at around 0.35 V during the discharge, while the discharge of catechol mainly proceed at around 0.65 V when silyl protecting groups are used during the modiﬁcation step. Note that by using unprotected catechol diazonium salt, the plateau is less well-deﬁned because the two reversible systems have approxi-mately the same current intensity. This change in potential for the faradaic contribution to the charge storage has a profound impact on the energy delivered at the discharge (Fig. 8). More the revers-ible electrochemical system at higher potential becomes pro-nounced, more the energy density increases. Whereas there is not much difference between the total speciﬁc charges with the two protected-catechol carbon products, the energy gain almost tripled with silyl groups compared to methyl groups, changing from 15% to 40%. These results make the bis((triisopropylsilyl)oxy)benzenedia-zonium salt a good candidate for the modiﬁcation of the Norit carbon for charge storage applications and prove that the molecular sizes must be adapted to the textural properties of porous carbons Table 1
Electrochemical performances of supercapacitors electrodes deduced from CVs at 10 mV s1.
Carbon products QT(C g1) Qdl(C g1) QF(C g1) GTGA(mol g1)a Faradaic efﬁciency (%)
Norit 114.6 114.6 e e e
Norit-OH 127.1 105.8 21.3 0.00125 8.8
Norit-OMe 136.4 107.9 28.5 0.00078 19.0 Norit-OTIPS 148.9 103.3 45.6 0.00040 59.0
aThe mass fraction of molecules is determined from the global weight loss at 700C.
Fig. 3. Evolution of the total speciﬁc charge as a function of scan rate for unmodiﬁed and modiﬁed Norit carbons.
Fig. 4. Adsorption-desorption isotherms of nitrogen at 77 K for unmodiﬁed and modiﬁed Norit carbons.
Fig. 5. Pore size distribution of unmodiﬁed and modiﬁed Norit carbons. The inset shows the subtracted pore volume distribution obtained by difference between the pore size distribution for the bis((triisopropylsilyl)oxy)benzene and dimethoxybenzene-modiﬁed Norit carbons.
to maximize the performances of carbon-molecules based hybrid storage systems.
Two different O-protected catechol diazonium salts were syn-thetized and introduced on the surface of the Norit-S50 carbon to prepare supercapacitor electrodes working in 1 M H2SO4. The
car-bon products obtained were characterized by TGA and XPS
experiments. After deprotection, multi-peak systems, mainly composed of two reversible systems separated by around 300 mV, were obtained in cyclic voltammetry. Results show that the relative intensities of these two pairs of symmetric peaks are related to the nature of the protecting group. The role of the protecting group and its impact on the potential at which catechol is electroactive after deprotection were investigated by electrochemical techniques and nitrogen gas adsorption-desorption measurements. The following conclusions can be drawn from results.
(i) The speciﬁc charge was improved by using a O-protected catechol diazonium salt with triisopropylsilyl groups during the modiﬁcation step.
(ii) With triisopropylsilyl protecting groups the reversible elec-trochemical system located at higher potential dominates, while that at lower potential mainly contributes to the multi-peak envelope in the CV when methyl protecting groups are used.
(iii) Due to a potential separation of around 300 mV between the two pairs of symmetric peaks, the speciﬁc energy gain delivered at the discharge at 1 A g1almost tripled by using triisopropylsilyl protecting groups, compared to the methyl groups.
(iv) The different locations in potential of the reversible elec-trochemical systems obtained in cyclic voltammetry seem mainly due to a textural effect. A tenable explanation is that the protection of catechol with bulky silyl groups does not allows the diffusion of the diazonium salt in the micropo-rosity, while the 3,4-dimethoxybenzenediazonium salt can Fig. 6. Schematic representation of the impact of the molecular size on the porous structure of the Norit carbon. In this representation, illustrated with the Norit-OTIPS carbon product, the normalized pore size distribution is obtained by dividing pore diameters d by the molecular size l, which is assumed to be the higher interatomic distance between the two protecting groups calculated by Chem3D.
Fig. 7. (A) Discharge curves at 1 A g1for unmodiﬁed and modiﬁed Norit carbon electrodes. (B) Evolution of the total speciﬁc charge during the ﬁrst 1100 charges/discharge cycles.
Fig. 8. Speciﬁc energy delivered during the discharge at 1 A g1for unmodiﬁed and
have access to a part of the micropores and can possibly reduce their volume by a progressive coverage of their inner surface.
The protection/deprotection strategy reported here could offer the possibility of matching a more important energy to the faradaic contribution of the electric charge storage in pseudo-supercapacitors just by adapting the textural properties of the activated carbon to the molecular size, without multi-step syn-thesis to prepare selected molecules.
This work was supported by the Centre National de la Recherche Scientiﬁque (CNRS-France) through the framework of the ICROSS project (ANR-13-PRGE-0011-02). We also thanks the French Min-istry for the PhD grant of E. Touze.
Appendix A. Supplementary data
Supplementary data related to this article can be found at
 K.W. Leitner, B. Gollas, M. Winter, J.O. Besenhard, Combination of redox ca-pacity and double layer capacitance in composite electrodes through immo-bilization of an organic redox couple on carbon black, Electrochim. Acta 50 (2004) 199e204.
 S. Isikli, R. Diaz, Substrate-dependent performance of supercapacitors based on an organic redox couple impregnated on carbon, J. Power Sources 206 (2012) 53e58.
 R.D.L. Smith, P.G. Pickup, Novel electroactive surface functionality from the coupling of an aryl diamine to carbon black, Electrochem. Commun. 11 (2009) 10e13.
 Z. Algharaibeh, X. Liu, P.G. Pickup, An asymmetric anthraquinone-modiﬁed carbon/ruthenium oxide supercapacitor, J. Power Sources 187 (2009) 640e643.
 K. Kalinathan, D.P. DesRoches, X. Liu, P.G. Pickup, Anthraquinone modiﬁed carbon fabric supercapacitors with improved energy and power densities, J. Power Sources 181 (2008) 182e185.
 M. Weissmann, O. Crosnier, T. Brousse, D. Belanger, Electrochemical study of anthraquinone groups, grafted by the diazonium chemistry, in different aqueous media-relevance for the development of aqueous hybrid electro-chemical capacitor, Electrochim. Acta 82 (2012) 250e256.
 L. Madec, A. Bouvree, P. Blanchard, C. Cougnon, T. Brousse, B. Lestriez,
D. Guyomard, J. Gaubicher, In situ redox functionalization of composite electrodes for high powerehigh energy electrochemical storage systems via a non-covalent approach, Energy Environ. Sci. 5 (2012) 5379e5386.  E. Lebegue, T. Brousse, O. Crosnier, J. Gaubicher, C. Cougnon, Direct
intro-duction of redox centers at activated carbon substrate based on acid-substituent-assisted diazotization, Electrochem. Commun. 25 (2012) 124e127.
 E. Lebegue, T. Brousse, J. Gaubicher, C. Cougnon, Chemical functionalization of
activated carbon through radical and diradical intermediates, Electrochem. Commun. 34 (2013) 14e17.
 S. Isikli, M. Lecea, M. Ribagorda, M.C. Carreno, R. Dıaz, Inﬂuence of quinone grafting via FriedeleCrafts reaction on carbon porous structure and super-capacitor performance, Carbon 66 (2014) 654e661.
 G. Pognon, T. Brousse, L. Demarconnay, D. Belanger, Performance and stability of electrochemical capacitor based on anthraquinone modiﬁed activated carbon, J. Power Sources 196 (2011) 4117e4122.
 A. Le Comte, G. Pognon, T. Brousse, D. Belanger, Determination of the quinone-loading of a modiﬁed carbon powder-based electrode for electrochemical capacitor, Electrochemistry 81 (2013) 863e866.
 Q. Abbas, P. Ratajczak, P. Babuchowska, A. Le Comte, D. Belanger, T. Brousse, F. Beguin, Strategies to improve the performance of carbon/carbon capacitors in salt aqueous electrolytes, J. Electrochem. Soc. 162 (2015) A5148eA5157.  X. Chen, H. Wang, H. Yi, X. Wang, X. Yan, Z. Guo, Anthraquinone on porous
carbon nanotubes with improved supercapacitor performance, J. Phys. Chem. C 118 (2014) 8262e8270.
 A. Le Comte, T. Brousse, D. Belanger, Simpler and greener grafting method for
improving the stability of anthraquinone-modiﬁed carbon electrode in alka-line media, Electrochim. Acta 137 (2014) 447e453.
 C. Cougnon, E. Lebegue, G. Pognon, Impedance spectroscopy study of a
catechol-modiﬁed activated carbon electrode as active material in electro-chemical capacitor, J. Power Sources 274 (2015) 551e559.
 Z. Algharaibeh, P.G. Pickup, An asymmetric supercapacitor with anthraqui-none and dihydroxybenzene modiﬁed carbon fabric electrodes, Electrochem. Commun. 13 (2011) 147e149.
 E. Lebegue, T. Brousse, J. Gaubicher, R. Retoux, C. Cougnon, Toward fully
organic rechargeable charge storage devices based on carbon electrodes grafted with redox molecules, J. Mater. Chem. 2 (2014) 8599e8602.  N. An, Y. An, Z. Hu, B. Guo, Y. Yang, Z. Lei, Graphene hydrogels non-covalently
functionalized with alizarin: an ideal electrode material for symmetric supercapacitors, J. Mater. Chem. 3 (2015) 22239e22246.
 X. Su, K.-J. Tan, J. Elbert, C. Rüttiger, M. Gallei, T.F. Jamison, T.A. Hatton, Asymmetric Faradaic systems for selective electrochemical separations, En-ergy Environ. Sci. 10 (2017) 1272e1283.
 C. Karlsson, E. J€amstorp, M. Strømme, M. Sj€odin, Computational electro-chemistry study of 16 isoindole-4,7-diones as candidates for organic cathode materials, J. Phys. Chem. C 116 (2012) 3793e3801.
 K. Herna
ndez-Burgos, S.E. Burkhardt, G.G. Rodríguez-Calero, R.G. Hennig, H.D. Abrunea, Theoretical studies of carbonyl-based organic molecules for energy storage applications: the heteroatom and substituent effect, J. Phys. Chem. C 118 (2014) 6046e6051.
 R.B. Araujo, A. Banerjee, P. Panigrahi, L. Yang, M. Strømme, M. Sj€odin,
C.M. Araujo, R. Ahuja, Designing strategies to tune reduction potential of organic molecules for sustainable high capacity battery application, J. Mater. Chem. 5 (2017) 4430e4454.
 S.E. Burkhardt, M.A. Lowe, S. Conte, W. Zhou, H. Qian, G.G. Rodriguez-Calero, J. Gao, R.G. Hennig, H.D. Abrunea, Tailored redox functionality of small organics for pseudocapacitive electrodes, Energy Environ. Sci. 5 (2012) 7176e7187.  G. Pognon, C. Cougnon, D. Mayilukila, D. Belanger, Catechol-modiﬁed
acti-vated carbon prepared by the diazonium chemistry for application as active electrode material in electrochemical capacitor, ACS Appl. Mater. Interfaces 4 (2012) 3788e3796.
 S. Uchiyama, H. Watanabe, H. Yamazaki, A. Kanazawa, H. Hamana, Y. Okabe, Electrochemical introduction of amino group to a glassy carbon surface by the electrolysis of carbamic acid, J. Electrochem. Soc. 154 (2007) F31eF35.  G.G. Wildgoose, A.T. Masheter, A. Crossley, J.H. Jones, R.G. Compton,
Elec-trolysis of ammonium carbamate: a voltammetric and X-ray photoelectron spectroscopic investigation into the modiﬁcation of carbon electrodes, Int. J. Electrochem. Sci. 2 (2007) 809e819.
 T. Nagaoka, T. Yoshino, Surface properties of electrochemically pretreated glassy carbon, Anal. Chem. 58 (1986) 1037e1042.
 A.S. Kumar, S. Sornambikai, P. Gayathri, J.-M. Zen, Selective covalent immo-bilization of catechol on activated carbon electrodes, J. Electroanal. Chem. 641 (2010) 131e135.
 A.S. Kumar, P. Swetha, Electrochemical-assisted encapsulation of catechol on a multiwalled carbon nanotube modiﬁed electrode, Langmuir 26 (2010) 6874e6877.
 S.A. Trammell, M. Moore, T.L. Schull, N. Lebedev, Synthesis and electro-chemistry of self-assembled monolayers containing quinone derivatives with varying electronic conjugation, J. Electroanal. Chem. 628 (2009) 125e133.  N.H. Nguyen, C. Cougnon, F. Gohier, Deprotection of arenediazonium
tetra-ﬂuoroborate ethers with BBr3, J. Org. Chem. 74 (2009) 3955e3957.
 M. Li, S.M.D. Shandilya, M.A. Carpenter, A. Rathore, W.L. Brown, A.L. Perkins, D.A. Harki, J. Solberg, D.J. Hook, K.K. Pandey, M.A. Parniak, J.R. Johnson, N.J. Krogan, M. Somasundaran, A. Ali, C.A. Schiffer, R.S. Harris, First-in-class small molecule inhibitors of the single-strand DNA cytosine deaminase APOBEC3G, ACS Chem. Biol. 7 (2012) 506e517.
 W.G. Hong, B.H. Kim, S.M. Lee, H.Y. Yu, Y.J. Yun, Y. Jun, J.B. Lee, H.J. Kim, Agent-free synthesis of graphene oxide/transition metal oxide composites and its application for hydrogen storage, Int. J. Hydrogen Energy 37 (2012) 7594e7599.
 A. Pendashteh, M.F. Mousavi, M.S. Rahmanifar, Fabrication of anchored copper oxide nanoparticles on graphene oxide nanosheets via an electrostatic coprecipitation and its application as supercapacitor, Electrochim. Acta 88 (2013) 347e357.
 M. Andresen, L.-S. Johansson, B.S. Tanem, P. Stenius, Properties and charac-terization of hydrophobized microﬁbrillated cellulose, Cellulose 13 (2006) 665e677.
 Y.R. Leroux, H. Fei, J.-M. No€el, C. Roux, P. Hapiot, Efﬁcient covalent
modiﬁca-tion of a carbon surface: use of a silyl protecting group to form an active monolayer, J. Am. Chem. Soc. 132 (2010) 14039e14041.
 M. Toupin, D. Belanger, Thermal stability study of aryl modiﬁed carbon black
by in situ generated diazonium salt, J. Phys. Chem. C 111 (2007) 5394e5401.  P. Doppelt, G. Hallais, J. Pinson, F. Podvorica, S. Verneyre, Surface modiﬁcation of conducting substrates. Existence of azo bonds in the structure of organic layers obtained from diazonium salts, Chem. Mater. 19 (2007) 4570e4575.  B.L. Hurley, R.L. McCreery, Covalent bonding of organic molecules to Cu and Al
alloy 2024 T3 surfaces via diazonium ion reduction, J. Electrochem. Soc. 151 (2004) B252eB259.
 L. Madec, K.A. Seid, J.-C. Badot, B. Humbert, P. Moreau, O. Dubrunfaut, B. Lestriez, D. Guyomard, J. Gaubicher, Redirected charge transport arising from diazonium grafting of carbon coated LiFePO4, Phys. Chem. Chem. Phys.
16 (2014) 22745e22753.
 G. Liu, E. Luais, J.J. Gooding, The fabrication of stable gold nanoparticle-modiﬁed interfaces for electrochemistry, Langmuir 27 (2011) 4176e4183.  P. Brant, R.D. Feltham, X-ray photoelectron spectra of aryldiazo derivatives of
 P. Finn, W.-L. Jolly, Nitrogen ls binding energies of some azide, dinitrogen, and nitride complexes of transition metals, Inorg. Chem. 11 (1972) 1434e1435.  T.M. Bockman, D. Kosynkin, J.K. Kochi, Isolation and structure elucidation of
transient (colored) complexes of arenediazonium with aromatic hydrocar-bons as intermediates in arylations and azo couplings, J. Org. Chem. 62 (1997) 5811e5820.
 T. Menanteau, M. Dias, E. Levillain, A.J. Downard, T. Breton, Electrografting via diazonium chemistry: the key role of the aryl substituent in the layer growth mechanism, J. Phys. Chem. C 120 (2016) 4423e4429.
 Y. Xie, P.M.A. Sherwood, X-ray photoelectron spectroscopic studies of carbon ﬁber surfaces. Differences in the surface chemistry and bulk structure of different carbonﬁbers based on poly(acrylonitrile) and pitch and comparison
with various graphite samples, Chem. Mater. 2 (1990) 293e299.
 Y.R. Leroux, P. Hapiot, Nanostructured monolayers on carbon substrates prepared by electrografting of protected aryldiazonium salts, Chem. Mater. 25 (2013) 489e495.
 J. Lehr, B.E. Williamson, A.J. Downard, Spontaneous grafting of nitrophenyl groups to planar glassy carbon substrates: evidence for two mechanisms, J. Phys. Chem. C 115 (2011) 6629e6634.
 K.S.W. Sing, D.H. Everett, R.A.W. Haul, L. Moscou, R.A. Pierotti, J. Rouquerol, T. Siemieniewska, Pure Appl. Chem. 57 (1985) 603e619.
 G. Pognon, T. Brousse, D. Belanger, Effect of molecular grafting on the pore size distribution and the double layer capacitance of activated carbon for elec-trochemical double layer capacitors, Carbon 49 (2011) 1340e1348.